Research Progress of TiO 2 Modification and Photodegradation of Organic Pollutants

: Titanium dioxide (TiO 2 ) photocatalysts, characterized by exceptional photocatalytic activity, high photoelectric conversion efficiency, and economic viability, have found widespread application in recent years for azo dye degradation. However, inherent constraints, such as the material’s limited visible light absorption stemming from its bandgap and the swift recombination of charge carriers, have impeded its broader application potential. Encouragingly, these barriers can be mitigated through the modification of TiO 2 . In this review, the common synthesis methods of TiO 2 are reviewed, and the research progress of TiO 2 modification technology at home and abroad is discussed in detail, including precious metal deposition, transition metal doping, rare earth metal doping, composite semiconductors, and composite polymers. These modification techniques effectively enhance the absorption capacity of TiO 2 in the visible region and reduce the recombination rate of carriers and electrons, thus significantly improving its photocatalytic performance. Finally, this paper looks forward to the future development direction of TiO 2 photocatalytic materials, including the exploration of new modified materials, in-depth mechanism research, and performance optimization in practical applications, to provide useful references for further research and application of TiO 2 photocatalytic materials.


Introduction
In recent years, acid rain, eutrophication of water bodies, black and smelly water bodies, PM2.5 exceeding standards, and other environmental issues have occurred frequently, warning us that environmental protection cannot be delayed.Among them, the content of organic pollutants and pigments is high, which seriously affects the regional water quality [1,2].Due to their highly stable structure and difficulty in handling, most of them are toxic to organisms, including direct lethality and carcinogenicity [3][4][5].This highlights the urgent need for effective treatment of pollutants in water, and the current treatment methods for organic pollutants are mainly the combination of physical, biochemical, and chemical treatment methods [6].
Physical treatment methods include adsorption, extraction, radiation-based techniques, and membrane separation [7][8][9].Biochemical treatment methods include aerobic treatment, anaerobic treatment [10,11], and so on.Chemical treatment methods include chemical oxidation, photocatalytic oxidation, electrochemical methods, chemical coagulation, and others [12][13][14].Although the traditional physical and chemical treatment methods can remove azo dyes to a certain extent, there are often problems such as high energy consumption, long treatment cycles, and secondary pollution.Therefore, the development of efficient and environmentally friendly treatment of water pollutants has become the focus of current research.As a new type of wastewater treatment technology being gradually developed based on photochemical oxidation [15], photocatalytic technology has garnered widespread favor among scholars due to its numerous advantages including good stability, high activity, non-toxicity, a wide range of applicability, and the absence of secondary pollution.Its ability to effectively degrade dye pollutants in water bodies is particularly noteworthy [16,17].Photocatalysts are primarily composed of n-type semiconductor materials, including TiO 2 , ZnO, CdS, and others.TiO 2 stands out as the most extensively studied and utilized n-type semiconductor material due to its exceptional chemical stability, non-toxicity, low cost, and strong photosensitivity [18,19].Its application areas span water treatment, air purification, solar cell photosensitizers, self-cleaning materials, and medical applications [20].In the degradation of organic pollutants in water, TiO 2 photocatalysis technology has shown unique advantages.TiO 2 photocatalyst can generate photogenerated electrons and holes under ultraviolet irradiation and then trigger a series of REDOX reactions.These reactions can break the chemical bonds of organic pollutant molecules and degrade them into small molecular compounds, ultimately achieving the purpose of removing the pollutants [21].
Although TiO 2 photocatalysis technology has many advantages in the degradation of pollutants in water, pure TiO 2 , with a band gap of 3.0~3.2eV [22], can only be excited by ultraviolet light with a wavelength less than 387 nm and photogenerated electronhole pairs are easy to recombine, resulting in low photo quantum efficiency and limited photocatalytic activity [23].To further improve the photocatalytic performance of TiO 2 , researchers modified TiO 2 through doping [24], composite, surface modification [25], and other means to optimize the structure of TiO 2 , thereby expanding its photoresponse range and reducing the carrier recombination rate [26,27].Thus, its application effect in the photodegradation of organic pollutants was enhanced.These modification methods can significantly improve the efficiency and performance of TiO 2 photocatalysts in degrading pollutants and provide better technical support for practical applications.In addition, the study of TiO 2 -modified photocatalysis technology has far-reaching significance [28].It not only helps to solve the environmental problems of organic pollutants such as azo dyes but also promotes the application and development of photocatalysis technology in other fields [29].Through in-depth research on the mechanism and methods of TiO 2 modification, theoretical guidance, and practical experience can be provided for the development of more efficient and environmentally friendly photocatalytic materials and contribute to environmental protection and sustainable development [30].

Mechanism of Photodegradation of Organic Pollutants by TiO 2 Photocatalyst
TiO 2 is a semiconductor, and its band structure is composed of a low-level valence band and a high-level conduction band [31].The valence band is mainly composed of 2p orbitals of oxygen atoms, and the conduction band is mainly composed of 3d, 4s, and 4p orbitals of titanium atoms [32].The band discontinuity of the semiconductor is bandgap between the valence band and the conduction band, and the energy difference between the conduction band and the valence band is called bandgap width [33].
TiO 2 mainly has three crystal structures, namely Anatase type, Rutile type, and Brookite type, of which rutile TiO 2 is the most stable crystal type, even at high temperatures will not be transformed and decomposed.The photocatalytic activity of anatase TiO 2 is higher than that of rutile TiO 2 because anatase TiO 2 has a lighter effective mass, smaller particle size, and longer life of photoexcited electrons and holes [34].As a metastable phase, titanite is rarely found in nature, is difficult to synthesize, and has low practical application value, so anatase-type TiO 2 is often used to photocatalyze the degradation of organic pollutants in water.For anatase phase TiO 2 , when it is irradiated by photons with energy greater than 3.2 eV (wavelength < 387.5 nm), the photoexcitation reaction will produce free electrons and holes: Excited electrons react with oxygen in the air to produce superoxide radical anions, which combine with water molecules to form hydroxyl radicals: (2) Hydroxyl radicals and superoxide radicals with strong oxidation react with organic pollutants, destroying their molecular structure; they are easily broken by oxidation.After a series of reactions, organic pollutant molecules are decomposed into harmless small molecules or low-toxicity compounds, such as water and carbon dioxide.The process is as follows: The photocatalytic mechanism of TiO 2 is depicted in Figure 1.
Inorganics 2024, 12, x FOR PEER REVIEW 3 of 23 organic pollutants in water.For anatase phase TiO2, when it is irradiated by photons with energy greater than 3.2 eV (wavelength < 387.5 nm), the photoexcitation reaction will produce free electrons and holes: Excited electrons react with oxygen in the air to produce superoxide radical anions, which combine with water molecules to form hydroxyl radicals: Hydroxyl radicals and superoxide radicals with strong oxidation react with organic pollutants, destroying their molecular structure; they are easily broken by oxidation.After a series of reactions, organic pollutant molecules are decomposed into harmless small molecules or low-toxicity compounds, such as water and carbon dioxide.The process is as follows: The photocatalytic mechanism of TiO2 is depicted in Figure 1.

Kinetics of Photodegradation of Organic Pollutants by TiO2 Photocatalyst
The photocatalytic degradation of organic pollutants by TiO2 is analyzed by the Langmuir-Hinshelwood model [35]; Arikal [36] et al. used chitosan as a carrier to immobilize TiO2/MgO nanocomposites on chitosan beads.MO and azo red S (ARS) were used as model dye compounds.The experimental results showed that the degradation of the pollutants followed first-order kinetics, and the Langmuir-Hinshelwood model was suitable for describing the kinetics of the photocatalytic degradation of wastewater.This is simplified as the first-order kinetics formula: In(C0/C) = kt, (C0) the initial concentration of organic pollutants, (C) the concentration of organic pollutants after degradation, (k) the apparent reaction rate constant, and (t) the photodegradation time.The model takes into account the adsorption and reaction processes on the catalyst surface and can describe the kinetic behavior of photocatalytic degradation well.The kinetics of photocatalytic degradation can be described by the degradation rate constant.The degradation rate constant reflects the relationship between degradation rate and pollutant concentration.
The influencing factors of reaction kinetics are as follows: • Solution pH value has an important effect on photocatalytic degradation.The photocatalytic activity of TiO2 may vary under acidic and alkaline conditions.

Kinetics of Photodegradation of Organic Pollutants by TiO 2 Photocatalyst
The photocatalytic degradation of organic pollutants by TiO 2 is analyzed by the Langmuir-Hinshelwood model [35]; Arikal [36] et al. used chitosan as a carrier to immobilize TiO 2 /MgO nanocomposites on chitosan beads.MO and azo red S (ARS) were used as model dye compounds.The experimental results showed that the degradation of the pollutants followed first-order kinetics, and the Langmuir-Hinshelwood model was suitable for describing the kinetics of the photocatalytic degradation of wastewater.This is simplified as the first-order kinetics formula: In(C 0 /C) = kt, (C 0 ) the initial concentration of organic pollutants, (C) the concentration of organic pollutants after degradation, (k) the apparent reaction rate constant, and (t) the photodegradation time.The model takes into account the adsorption and reaction processes on the catalyst surface and can describe the kinetic behavior of photocatalytic degradation well.The kinetics of photocatalytic degradation can be described by the degradation rate constant.The degradation rate constant reflects the relationship between degradation rate and pollutant concentration.
The influencing factors of reaction kinetics are as follows: • Solution pH value has an important effect on photocatalytic degradation.The photocatalytic activity of TiO 2 may vary under acidic and alkaline conditions.• The amount of catalyst dosing will also affect the degradation rate.Less than or more than the optimal dosage will lead to a decrease in the degradation rate.

•
Factors such as organic pollutant's initial concentration and light intensity also affect the kinetic process of photocatalytic degradation.
In summary, the process of photodegradation of organic pollutants using TiO 2 photocatalyst involves complex chemical reactions and kinetic behaviors.Through an in-depth understanding of its mechanism and kinetics, the photocatalytic degradation process can be optimized, and the degradation efficiency and environmental protection effect can be improved.

Synthesis Method of TiO 2 Photocatalyst
As a functional material, TiO 2 has high photocatalytic activity and, therefore, has an excellent advantage in the field of photocatalytic degradation.At present, the methods commonly used to synthesize TiO 2 include the sol-gel method, hydrothermal method, atomic layer deposition method, and microemulsion method.In terms of structure and morphology, a variety of morphologically controllable TiO 2 micro-nano meters, such as nanorods, nanotubes, nano-flowers, nano-hollow spheres, and mesoporous structures, were prepared through various experiments.As shown in Figure 2, these micro-nano TiO 2 materials with large specific surface areas usually have more excellent photocatalytic properties.

•
Factors such as organic pollutant's initial concentration and light intensity also affect the kinetic process of photocatalytic degradation.
In summary, the process of photodegradation of organic pollutants using TiO2 photocatalyst involves complex chemical reactions and kinetic behaviors.Through an indepth understanding of its mechanism and kinetics, the photocatalytic degradation process can be optimized, and the degradation efficiency and environmental protection effect can be improved.

Synthesis Method of TiO2 Photocatalyst
As a functional material, TiO2 has high photocatalytic activity and, therefore, has an excellent advantage in the field of photocatalytic degradation.At present, the methods commonly used to synthesize TiO2 include the sol-gel method, hydrothermal method, atomic layer deposition method, and microemulsion method.In terms of structure and morphology, a variety of morphologically controllable TiO2 micro-nano meters, such as nanorods, nanotubes, nano-flowers, nano-hollow spheres, and mesoporous structures, were prepared through various experiments.As shown in Figure 2, these micro-nano TiO2 materials with large specific surface areas usually have more excellent photocatalytic properties.

Sol-Gel Method
Sol-gel is the most commonly used process method for preparing TiO2 photocatalytic materials [38].Inorganic salts and Alkoxides (including tetraethyl titanate, butyl titanate, isopropanol titanium, etc.) are placed in distilled water, mixed evenly at room temperature under liquid phase conditions, and a stable, transparent sol system is formed in solution through chemical reaction steps such as hydrolysis and condensation, as shown in Figure 3.After aging for some time, the colloidal gel slowly polymerizes to form a wet gel with a three-dimensional network structure, and the gel network is filled with solvent that

Sol-Gel Method
Sol-gel is the most commonly used process method for preparing TiO 2 photocatalytic materials [38].Inorganic salts and Alkoxides (including tetraethyl titanate, butyl titanate, isopropanol titanium, etc.) are placed in distilled water, mixed evenly at room temperature under liquid phase conditions, and a stable, transparent sol system is formed in solution through chemical reaction steps such as hydrolysis and condensation, as shown in Figure 3.After aging for some time, the colloidal gel slowly polymerizes to form a wet gel with a three-dimensional network structure, and the gel network is filled with solvent that loses fluidity.The wet gel is prepared by vacuum drying, high-temperature roasting, and curing to produce molecular and even nanostructured materials.Nanomaterials prepared by the sol-gel method have the advantages of high purity, uniformity, and controllable morphology and have been widely used in the preparation of TiO 2 .
loses fluidity.The wet gel is prepared by vacuum drying, high-temperature roasting, and curing to produce molecular and even nanostructured materials.Nanomaterials prepared by the sol-gel method have the advantages of high purity, uniformity, and controllable morphology and have been widely used in the preparation of TiO2.Jamil [39], Huo [40], Fermeli [41], et al. prepared a composite photocatalyst by sol-gel method.The results show that the prepared TiO2 composite photocatalyst has good dispersibility, a large specific surface area, and good photocatalytic activity.Dinkar Parashar [42] prepared photocatalysts by sol-gel method at different calcination temperatures (400-800 °C) and hydroalcohol ratios.The activity of TiO2 prepared by the sol-gel method was higher than that of commercially available pure anatase TiO2 nanoparticles due to the smaller average particle size.It was found that the ratio of water to alcohol in the preparation of TiO2 catalysts had a significant effect on antibiotic removal.Namely, the removalrate constants of metronidazole (MNZ), ciprofloxacin (CIP), and tetracycline (TET) were improved by a factor of 2.7, 3.3, and 1.6, which further indicates that the sol-gel prepared TiO2 can effectively remove the harmful substance.Lalitha [43] et al. synthesized TiO2/ZnO with quadrilateral and hexagonal structures by sol-gel method; the catalyst displayed 90% degradation within 40 min under UV light conditions.

Hydrothermal Synthesis
The hydrothermal synthesis method is a reaction occurring at high temperature and high pressure [44], which uses water or organic solvent as a medium through heating so that insoluble or insoluble substances are dissolved or recrystallized after washing and centrifugation to obtain the required nanoparticle.Rawat [45], Matakgane [46], et al. prepared composite photocatalysts by hydrothermal method.The results of photocatalytic performance show that it has good absorption ability to ultraviolet light and good transmittibility to visible light.Yang [47] et al. synthesized a novel 3D sea urchin-type titanium dioxide by the EDTA-Na2-assisted hydrothermal method (Figure 4).Benefiting from the conical structure prepared by the hydrothermal method and the rapid separation of photogenerated electron holes in the mixed crystal phase, the sub-micron-sized 3D sea urchintype titanium dioxide can efficiently degrade 94.1% of the methicillin in the aqueous solution in 90 min, which is superior to that of the commercially available 25 nm-sized rutile titanium dioxide.Zhang [48] et al. modified TiO2 with a carboxyl group and amino group by hydrothermal method, making the adsorption performance of functionalized TiO2 better than P25 (unmodified commercial TiO2).Moreover, the functionalized TiO2 has good reusability for the removal of azo dye acid red G even after 5 adsorption-desorption cycles.Jamil [39], Huo [40], Fermeli [41], et al. prepared a composite photocatalyst by sol-gel method.The results show that the prepared TiO 2 composite photocatalyst has good dispersibility, a large specific surface area, and good photocatalytic activity.Dinkar Parashar [42] prepared photocatalysts by sol-gel method at different calcination temperatures (400-800 • C) and hydroalcohol ratios.The activity of TiO 2 prepared by the sol-gel method was higher than that of commercially available pure anatase TiO 2 nanoparticles due to the smaller average particle size.It was found that the ratio of water to alcohol in the preparation of TiO 2 catalysts had a significant effect on antibiotic removal.Namely, the removal-rate constants of metronidazole (MNZ), ciprofloxacin (CIP), and tetracycline (TET) were improved by a factor of 2.7, 3.3, and 1.6, which further indicates that the sol-gel prepared TiO 2 can effectively remove the harmful substance.Lalitha [43] et al. synthesized TiO 2 /ZnO with quadrilateral and hexagonal structures by sol-gel method; the catalyst displayed 90% degradation within 40 min under UV light conditions.

Hydrothermal Synthesis
The hydrothermal synthesis method is a reaction occurring at high temperature and high pressure [44], which uses water or organic solvent as a medium through heating so that insoluble or insoluble substances are dissolved or recrystallized after washing and centrifugation to obtain the required nanoparticle.Rawat [45], Matakgane [46], et al. prepared composite photocatalysts by hydrothermal method.The results of photocatalytic performance show that it has good absorption ability to ultraviolet light and good transmittibility to visible light.Yang [47] et al. synthesized a novel 3D sea urchin-type titanium dioxide by the EDTA-Na2-assisted hydrothermal method (Figure 4).Benefiting from the conical structure prepared by the hydrothermal method and the rapid separation of photogenerated electron holes in the mixed crystal phase, the sub-micron-sized 3D sea urchin-type titanium dioxide can efficiently degrade 94.1% of the methicillin in the aqueous solution in 90 min, which is superior to that of the commercially available 25 nm-sized rutile titanium dioxide.Zhang [48] et al. modified TiO 2 with a carboxyl group and amino group by hydrothermal method, making the adsorption performance of functionalized TiO 2 better than P25 (unmodified commercial TiO 2 ).Moreover, the functionalized TiO 2 has good reusability for the removal of azo dye acid red G even after 5 adsorption-desorption cycles.
With the progress of scientific research, the hydrothermal method has attracted more and more attention from researchers, especially hydrothermal crystal growth, which has become the focus of research and will become the development object of the scientific research community.Hydrothermal preparation of nanomaterials equipment and conditions still need to be further explored and studied.With the progress of scientific research, the hydrothermal method has attracted more and more attention from researchers, especially hydrothermal crystal growth, which has become the focus of research and will become the development object of the scientific research community.Hydrothermal preparation of nanomaterials equipment and conditions still need to be further explored and studied.

Atomic Layer Deposition Method
Atomiclayer deposition (ALD) technology, also known as Atomiclayer epitaxy (ALE) technology, is a chemical vapor deposition technology based on ordered surface autosaturation reactions.Generally speaking, it is a method of coating the material layer by layer on the substrate surface in the form of a single atomic film.Jialin [49], Abidi [50], et al. used the atomic deposition method to prepare TiO2 and found that the prepared TiO2 nanoparticles were still anatase-type at high temperatures, had particularly good dispersion, and had high photocatalytic activity after degrading dyes.Cao [51] et al. modified the ultra-thin Fe2O3 layer of industrial anatase TiO2 powder by atomic layer deposition (ALD).The ultra-thin Fe2O3 coating with a small band gap of 2.20 eV can increase the visible light absorption of the TiO2 carrier, and the degradation efficiency of TiO2 powder coated with ALD Fe2O3 is the highest within 90 min, reaching 97.4%.Feng [52] et al. used atomic layer deposition (ALD) to deposit TiO2 nanoparticles on carbon nanotube membranes to prepare hydrophilic electrodes, as shown in Figure 5.After 20 ALD cycles, the modified carbon nanotube membranes showed better electrosorption performance and reusability in the CDI process.The total Cr and Cr(VI) removal significantly increased to 92.1% and 93.3%, respectively.This work demonstrates that ALD is a highly controllable and simple method for the preparation of advanced CDI electrodes, broadening the application of metal oxide/carbon composites in electrochemical processes, especially in the field of photocatalytic degradation of organic pollutants.

Atomic Layer Deposition Method
Atomiclayer deposition (ALD) technology, also known as Atomiclayer epitaxy (ALE) technology, is a chemical vapor deposition technology based on ordered surface autosaturation reactions.Generally speaking, it is a method of coating the material layer by layer on the substrate surface in the form of a single atomic film.Jialin [49], Abidi [50], et al. used the atomic deposition method to prepare TiO 2 and found that the prepared TiO 2 nanoparticles were still anatase-type at high temperatures, had particularly good dispersion, and had high photocatalytic activity after degrading dyes.Cao [51] et al. modified the ultra-thin Fe 2 O 3 layer of industrial anatase TiO 2 powder by atomic layer deposition (ALD).The ultra-thin Fe 2 O 3 coating with a small band gap of 2.20 eV can increase the visible light absorption of the TiO 2 carrier, and the degradation efficiency of TiO 2 powder coated with ALD Fe 2 O 3 is the highest within 90 min, reaching 97.4%.Feng [52] et al. used atomic layer deposition (ALD) to deposit TiO 2 nanoparticles on carbon nanotube membranes to prepare hydrophilic electrodes, as shown in Figure 5.After 20 ALD cycles, the modified carbon nanotube membranes showed better electrosorption performance and reusability in the CDI process.The total Cr and Cr(VI) removal significantly increased to 92.1% and 93.3%, respectively.This work demonstrates that ALD is a highly controllable and simple method for the preparation of advanced CDI electrodes, broadening the application of metal oxide/carbon composites in electrochemical processes, especially in the field of photocatalytic degradation of organic pollutants.With the progress of scientific research, the hydrothermal method has attracted more and more attention from researchers, especially hydrothermal crystal growth, which has become the focus of research and will become the development object of the scientific research community.Hydrothermal preparation of nanomaterials equipment and conditions still need to be further explored and studied.

Atomic Layer Deposition Method
Atomiclayer deposition (ALD) technology, also known as Atomiclayer epitaxy (ALE) technology, is a chemical vapor deposition technology based on ordered surface autosaturation reactions.Generally speaking, it is a method of coating the material layer by layer on the substrate surface in the form of a single atomic film.Jialin [49], Abidi [50], et al. used the atomic deposition method to prepare TiO2 and found that the prepared TiO2 nanoparticles were still anatase-type at high temperatures, had particularly good dispersion, and had high photocatalytic activity after degrading dyes.Cao [51] et al. modified the ultra-thin Fe2O3 layer of industrial anatase TiO2 powder by atomic layer deposition (ALD).The ultra-thin Fe2O3 coating with a small band gap of 2.20 eV can increase the visible light absorption of the TiO2 carrier, and the degradation efficiency of TiO2 powder coated with ALD Fe2O3 is the highest within 90 min, reaching 97.4%.Feng [52] et al. used atomic layer deposition (ALD) to deposit TiO2 nanoparticles on carbon nanotube membranes to prepare hydrophilic electrodes, as shown in Figure 5.After 20 ALD cycles, the modified carbon nanotube membranes showed better electrosorption performance and reusability in the CDI process.The total Cr and Cr(VI) removal significantly increased to 92.1% and 93.3%, respectively.This work demonstrates that ALD is a highly controllable and simple method for the preparation of advanced CDI electrodes, broadening the application of metal oxide/carbon composites in electrochemical processes, especially in the field of photocatalytic degradation of organic pollutants.Furthermore, Ostyn et al. [53] prepared TiO 2 film on graphene with ALD and oxidized the surface of graphite.The film has a high UV transmittance of 95%, which simplifies the experimental design.No chemical reagents are used to reduce the risk of contamination.TiO 2 films prepared by ALD react rapidly in graphite photooxidation, which is superior to traditional powder photocatalysts.Ke et al. [54] grew TiO 2 films by depositing atomic layers on silica support (SBA-15) and depositing precious metal Au on them and found that titanium dioxide films can successfully grow on mesoporous materials, increasing the specific surface area of the catalyst.Lys et al. [55] successfully combined laser-induced Si nano-fringes (SiNR), MXene, and TiO 2 to produce efficient ternary photocatalytic materials through ALD technology.Experiments show that the material has strong absorption capacity in the spectrum range, high stability, repeatability, and photocatalytic efficiency, which provides a new way for the photodegradation of azo dyes in wastewater treatment and shows broad application prospects.

Microemulsion Method
The microemulsion method is used for the preparation of nano or polymeric materials by adding surfactants and co-solvents and mixing the immiscible solution into a homogeneous phase [56].Its advantage is that it can prepare nano-sized and highly dispersible materials with mild conditions and high-quality performance.Because of the large interfacial area and high surface activity of microemulsion, it can improve the reaction efficiency and yield, which is widely used in the preparation of nanomaterials, polymer materials, and catalysts.
Sun [57] et al. prepared Fe 3 O 4 @TiO 2 composite photocatalyst by microemulsionsolvothermal method.It was found that Fe 3 O 4 @TiO 2 could reduce the band gap, and the degradation rates of Fe 3 O 4 @TiO 2 and TiO 2 for acid red 73 were 93.56% and 74.47%, respectively.Yang [58] et al. successfully prepared TiO 2 nanofibers with porous and mixedcrystal structures by the microemulsion method, which can directly regulate the structure of titanium dioxide nanofibers by changing the microemulsion system.The titanium dioxide obtained by the microemulsion method shows a porous and mixed-crystal structure and excellent photocatalytic properties.It is simple to prepare and is of great importance for the application of the preparation and enhancement of the performance of the special-shape photocatalytic materials.The degradation rate of methylene blue solution was as high as 98% after 90 min, which was effective in the treatment of printing and dyeing wastewater.
However, the microemulsion method also has limitations that include the following: the product purity is not high, the reagent is difficult to completely remove, the precursor must be water-soluble or oil-soluble, and the preparation and control of the microemulsion is complicated, which requires experimental experience and technical skill.

Other Synthesis Methods
In addition to the above four most common methods for synthesizing TiO 2 , there is also the Suzuki coupling reaction method [59], the electrostatic spinning method [60], the one-pot method [61], etc. Suzuki coupling reaction is a palladium-catalyzed crosscoupling reaction of aryl or alkenyl boronic acids or boronic esters with chlorine, bromine, iodine-substituted aromatic hydrocarbons or olefins.The one-pot method is a method in which the reactants are made to undergo successive multi-step reactions in a single reactor to improve the reaction efficiency.TiO 2 preparation by electrostatic spinning is a method of stretching titanium-containing solution into fibers using a high-voltage electric field, followed by heat treatment to obtain TiO 2 nanofibers.Djeda [62] et al. prepared layered double hydroxide (LDH)/TiO 2 nanocomposites with photocatalytic properties by immersion and direct coprecipitation methods and compared them with pure TiO 2 colloidal solutions.The degradation experiments showed that MgAl LDH/TiO 2 prepared by the coprecipitation method had the highest photodegradation efficiency for Orange II, which emphasized the importance of the preparation method of nanocomposites.Suitable synthesis methods can be selected according to different application requirements.
In summary, the most commonly used synthesis methods of TiO 2 photocatalysts, their reaction principles, and their advantages and disadvantages are shown in Table 1.Combined with the advantages and disadvantages of the four preparation methods-the sol-gel method, hydrothermal method, microemulsion method, and atomic deposition method-the improvement measures of TiO 2 preparation in the future can be focused on improving the preparation efficiency, reducing the cost, optimizing the performance, and meeting specific application needs.Through the above different preparation methods, two or more preparation methods can be combined according to the need to prepare the new, more stable, and higher photocatalytic efficiency of terpolymer or multi-component modified TiO 2 photocatalytic materials.

Modification Method of TiO 2 Photocatalyst
The direct preparation of TiO 2 sols can effectively solve the application challenges of TiO 2 particles, such as easy agglomeration and difficult loading [63].However, TiO 2 nanocrystals in sol still face the problems of limited photoresponse range and high carrier complexation rate.To further enhance its photocatalytic performance, it is necessary to broaden the light absorption range of TiO 2 nanocrystalline sols and improve the separation efficiency of their photogenerated carriers by various modification methods.

Precious Metal-Doped Titanium Dioxide
Precious metals and TiO 2 have different Fermi energy levels, and the work function of the metal is higher than that of the semiconductor TiO 2 ; electrons usually tend to flow from the semiconductor to the metal when the two are in contact [64].This cross-interface migration of electrons contributes to the efficient separation of electrons and holes in the semiconductor, as shown in Figure 6 Therefore, noble metals such as gold (Au), silver (Ag), platinum (Pt), and palladium (Pd) can significantly enhance the photocatalytic activity of TiO 2 materials [65].In these applications, noble metal nanoparticles play a key role in trapping or transferring photogenerated electrons [66].
Inorganics 2024, 12, x FOR PEER REVIEW 9 of 23 activity of TiO2 materials [65].In these applications, noble metal nanoparticles play a key role in trapping or transferring photogenerated electrons [66].The precious metal silver is relatively cheap and readily available [68].Several studies, such as Chacon-Argaez [69], Borrego Pérez [70], etc., have found that the photocatalytic activity of composites is indeed significantly improved.Mohammed, W [71] et al. found that Schottky promoted electron transfer at Ag-TiO2, transferred the absorption to the visible region, reduced the band gap of TiO2, and inhibited electron-hole recombination, thus enhancing the photocatalytic activity and stability.
Other precious metal deposits, such as Wang et al. [72] promoted the interaction between Pt and TiO2 by introducing oxygen vacancies through the carrier material, which facilitated the charge transfer from the carrier to Pt and exhibited excellent redox properties.Liu et al. [73] successfully prepared Au-TiO2 nanoparticles by the hydrothermal synthesis method and found that the optical band gap value of the composites decreased due to the doping of Au or the formation of oxygen vacancies, etc., which induced a narrowing of the Au-TiO2 band gap and increased visible light absorption, thus effectively degrading the MB.
The noble metal nanoparticles have a high specific surface area, good surface activity, and small particle size, which are characteristic of multiphase catalysis [74,75].However, the catalytic activity may be limited by the limited ability of noble metals to absorb light at specific wavelengths [76,77].In addition, the precious metal deposited TiO2 is less efficient in utilizing visible light and requires higher energy of UV light for better catalytic effect.However, precious metals are expensive resources, and doping them into TiO2 also increases the processing cost, which may be less economical in large-scale applications.

Transition Metal-Doped Titanium Dioxide
Interestingly, doping a moderate amount of transition metal ions in TiO2, the electrons in the d-and f-orbitals can undergo a transition and enter into the TiO2 structure, which reduces the bandgap and shifts the absorption edge to the visible region and reduces the rate of carrier complexation, thus improving the photocatalytic efficiency of TiO2 [78].At present, the transition metal doped ions are applied more: iron (Fe 3+ ), copper (Cu 2+ ), manganese (Mn 2+ ), vanadium (V 4+ ), zinc (Zn 2+) , etc [79].

Doping with a Single Transition Metal Elements
When TiO2 is doped with a single transition metal ion, the addition of the transition metal elements will change the lattice structure of TiO2 and thus its crystal crystallinity since they have multiple valences.This change affects the compounding process of photogenerated electrons and holes, thus improving the photocatalytic activity.Meshram et al. [80] microwave synthesized TiO2-Al composite photocatalysts and found that the The precious metal silver is relatively cheap and readily available [68].Several studies, such as Chacon-Argaez [69], Borrego Pérez [70], etc., have found that the photocatalytic activity of composites is indeed significantly improved.Mohammed, W [71] et al. found that Schottky promoted electron transfer at Ag-TiO 2 , transferred the absorption to the visible region, reduced the band gap of TiO 2, and inhibited electron-hole recombination, thus enhancing the photocatalytic activity and stability.
Other precious metal deposits, such as Wang et al. [72] promoted the interaction between Pt and TiO 2 by introducing oxygen vacancies through the carrier material, which facilitated the charge transfer from the carrier to Pt and exhibited excellent redox properties.Liu et al. [73] successfully prepared Au-TiO 2 nanoparticles by the hydrothermal synthesis method and found that the optical band gap value of the composites decreased due to the doping of Au or the formation of oxygen vacancies, etc., which induced a narrowing of the Au-TiO 2 band gap and increased visible light absorption, thus effectively degrading the MB.
The noble metal nanoparticles have a high specific surface area, good surface activity, and small particle size, which are characteristic of multiphase catalysis [74,75].However, the catalytic activity may be limited by the limited ability of noble metals to absorb light at specific wavelengths [76,77].In addition, the precious metal deposited TiO 2 is less efficient in utilizing visible light and requires higher energy of UV light for better catalytic effect.However, precious metals are expensive resources, and doping them into TiO 2 also increases the processing cost, which may be less economical in large-scale applications.

Transition Metal-Doped Titanium Dioxide
Interestingly, doping a moderate amount of transition metal ions in TiO 2 , the electrons in the d-and f-orbitals can undergo a transition and enter into the TiO 2 structure, which reduces the bandgap and shifts the absorption edge to the visible region and reduces the rate of carrier complexation, thus improving the photocatalytic efficiency of TiO 2 [78].At present, the transition metal doped ions are applied more: iron (Fe 3+ ), copper (Cu 2+ ), manganese (Mn 2+ ), vanadium (V 4+ ), zinc (Zn 2+) , etc [79].

Doping with a Single Transition Metal Elements
When TiO 2 is doped with a single transition metal ion, the addition of the transition metal elements will change the lattice structure of TiO 2 and thus its crystal crystallinity since they have multiple valences.This change affects the compounding process of photogenerated electrons and holes, thus improving the photocatalytic activity.Meshram et al. [80] microwave synthesized TiO 2 -Al composite photocatalysts and found that the surface area and porosity of the composites were significantly reduced compared to their pristine components and were successfully used for the degradation of mixed azodyes such as methylene blue and rhodamine B. Zhu et al. [81] prepared iron-doped TiO 2 thin films, and concluded that the right amount of iron ions effectively inhibited the composite to enhance the photogeneration of the rate of electron holes and that the enhanced photoactivity of Fe-doped TiO 2 samples was due to the generation of new elements to generate electronic states within the TiO 2 band gap.Mingmongkol et al. [82] prepared TiO 2 -doped composite photocatalysts with transition metal Cu and found that Cu doping did not cause any difference in the particle size or specific surface area, and on the other hand, the surface of the TiO 2 material doped with high concentration of Cu charge transfer had a negative effect.Cu-doped TiO 2 showed much greater photocatalytic degradation of methylene blue compared to undoped TiO 2 .

Co-Doping of Transition Metal Elements
In contrast, co-doping transition metals may produce more complex effects.Co-doping implies the simultaneous introduction of two or more different transition metal ions into TiO 2 .Co-doping may further enhance the efficiency of photogenerated electron-hole separation through synergistic effects or broaden the light absorption range of TiO 2 by introducing new energy levels.Rao et al. [83] prepared Cu and Zn co-doped TiO 2 nano-photocatalysts and found that the addition of Cu and Zn to TiO 2 hindered the growth of nanoparticles, and there existed a more efficient electron-hole generation.Sukhadeve et al. [84] prepared Zn and Fe co-doped TiO 2 nanoparticles using a simple sol-gel process, and the absorption spectra of the prepared nanoparticles showed strong absorption in visible light.The synergistic effect produced by Zn and Fe blocked the photoinduced charge carriers and delayed the complexation probability, which greatly improved the RhB, MG, and MB mixture pollution degradation efficiency.
Transition metal elements have multiple valence, which can promote the chemical reaction in the electronic conduction of TiO 2 , but it is worth noting that the doping amount should be controlled.Otherwise, it is not conducive to the improvement of the catalytic performance, and dopants are prone to agglomeration [85], such as the surface of the enriched or even the formation of new phases, so that the effective surface area of the semiconductor material is reduced, resulting in a decrease in the activity [86].

Rare Earth Metal-Doped Titanium Dioxide
Due to their unique electronic orbital structure [87], the doping of rare earth metal ions can adjust the energy level structure of TiO 2 , enabling it to absorb more light within the visible light range and thus enhancing photocatalytic activity [88].Additionally, rare earth metal doping can introduce additional energy levels, promoting the separation of photogenerated electrons and holes [89].It can also improve the photostability of titanium dioxide, enhancing its long-term stability and extending the lifespan of photocatalytic materials [90].This opens up new possibilities for its application in environmental purification, water treatment, energy conversion, and other fields [91].Common rare earth metals used for doping include ytterbium, erbium, holmium, lan, cerium, yttrium, and europium [92].

Doping with a Single Rare Earth Metal Element
Single rare earth element doped TiO 2 is relatively easy to synthesize and can be more easily achieved in the TiO 2 lattice for control and regulation [93].Ćurković et al. [94] prepared ce doped TiO 2 nanocomposites by sol-gel method and found that the absorption of the composites in the visible light band was higher than that of pure TiO 2 nanomaterials, and three cycles could be reused.Ikram Benammar et al. [95] used a hydrothermal-assisted sol-gel-gel method to prepare rare earth ytterbium and erbium-doped TiO 2 , respectively, and the optical properties were improved after heat treatment of the powders and downconversion of erbium-doped nanoparticles was observed.

Co-Doping with Rare Earth Metal Elements
Single transition metal element doping may not be able to fully optimize the energy band structure of TiO 2 [96], while rare earth element co-doping can extend the light absorption range of TiO 2 , enabling it to absorb wider wavelength bands of light [97], enhancing the light absorption capacity and photoelectric conversion efficiency of TiO 2 , and improving the stability of the catalyst surface [98].
Pascariu [99] et al. used electrospinning calcination of normal TiO 2 doped with Sm 3+ and Er 3+ to demonstrate the stability and reusability of the catalyst in five repeated cycles of photodegradation of MB.Guetni et al. [100] designed a new co-doped TiO 2 with Nd-Sm and La/Y apatite nanoparticles, which showed the highest degradation rate of 96.49% for azo dye Orange Yellow G within 105 min.Ren et al. [101] used the classical sol-gel method to prepare TiO 2 nanoparticles co-doped with rare earth elements Ce and Er, as shown in Figure 7.The composite photocatalyst is a spherical particle with an uneven radius.It can be seen in Figure 7c that the polyhedral structure is mainly composed of hexagons and rhomboids, with an average size of 30 nm.The results show that Ce doping can reduce the band gap width of the composite and give it the ability to respond to visible light.At the same time, the upconversion luminescence characteristics of Er can convert near-infrared light in the solar spectrum into short-wave light that is more easily absorbed by TiO 2 , thus enhancing the utilization rate of sunlight by the material.In addition, the doping of these two rare earth elements can effectively promote the separation and migration of photogenerated electrons and holes and optimize carrier utilization efficiency.Therefore, doped TiO 2 nanoparticles show better photocatalytic performance.
respectively, and the optical properties were improved after heat treatment of the powders and down-conversion of erbium-doped nanoparticles was observed.

Co-Doping with Rare Earth Metal Elements
Single transition metal element doping may not be able to fully optimize the energy band structure of TiO2 [96], while rare earth element co-doping can extend the light absorption range of TiO2, enabling it to absorb wider wavelength bands of light [97], enhancing the light absorption capacity and photoelectric conversion efficiency of TiO2, and improving the stability of the catalyst surface [98].
Pascariu [99] et al. used electrospinning calcination of normal TiO2 doped with Sm 3+ and Er 3+ to demonstrate the stability and reusability of the catalyst in five repeated cycles of photodegradation of MB.Guetni et al. [100] designed a new co-doped TiO2 with Nd-Sm and La/Y apatite nanoparticles, which showed the highest degradation rate of 96.49% for azo dye Orange Yellow G within 105 min.Ren et al. [101] used the classical sol-gel method to prepare TiO2 nanoparticles co-doped with rare earth elements Ce and Er, as shown in Figure 7.The composite photocatalyst is a spherical particle with an uneven radius.It can be seen in Figure 7c that the polyhedral structure is mainly composed of hexagons and rhomboids, with an average size of 30 nm.The results show that Ce doping can reduce the band gap width of the composite and give it the ability to respond to visible light.At the same time, the upconversion luminescence characteristics of Er can convert near-infrared light in the solar spectrum into short-wave light that is more easily absorbed by TiO2, thus enhancing the utilization rate of sunlight by the material.In addition, the doping of these two rare earth elements can effectively promote the separation and migration of photogenerated electrons and holes and optimize carrier utilization efficiency.Therefore, doped TiO2 nanoparticles show better photocatalytic performance.

Co-Doping of Rare Earth Elements with Other Elements
Co-doping of rare earth elements with other elements has also attracted extensive research [102,103].Li Jia et al. [104] synthesized lanthanum, graphene oxide (GO), and TiO2 by sol-gel method to prepare an efficient photocatalytic material with visible light

Co-Doping of Rare Earth Elements with Other Elements
Co-doping of rare earth elements with other elements has also attracted extensive research [102,103].Li Jia et al. [104] synthesized lanthanum, graphene oxide (GO), and TiO 2 by sol-gel method to prepare an efficient photocatalytic material with visible light response.Lattice distortion occurred in the samples added with the rare earth element lanthanum, which increased the surface area of the photocatalyst and significantly improved the photocatalytic activity of TiO 2 .The degradation efficiency of acid red B reached 95.6% after 5 h of simulated sunlight irradiation.
Co-doping of rare earth elements with other elements increases the separation efficiency of photogenerated electron-hole pairs and the number of surface active sites and improves the utilization efficiency of visible and infrared light.However, the co-doping of rare earth elements with other elements involves the synthesis and control of multi-element systems, so the preparation process and conditions are more complicated [105,106].

Compound Semiconductors Based on Titanium Dioxide
Semiconductor compounding is a method used to enhance photocatalytic efficiency by combining different types of semiconductor materials to form heterojunctions, as exemplified in Figure 8, which depicts a p-n heterojunction formed by TiO 2 and ZnO.The semiconductor composite effectively improves photocatalytic efficiency due to the following advantages: By manipulating the size of the modified particles, the spectral absorption range and bandgap of the semiconductor material can be effectively tuned utilizing the quantum size effect [107,108].2.
Surface modification of TiO 2 plays a role in improving the photostability of the semiconductor materials [109].

3.
Given that light absorption in semiconductors mainly occurs at the band-edge, the semiconductor composite facilitates more efficient harvesting of sunlight [110].
95.6% after 5 h of simulated sunlight irradiation.Co-doping of rare earth elements with other elements increases the separation efficiency of photogenerated electron-hole pairs and the number of surface active sites and improves the utilization efficiency of visible and infrared light.However, the co-doping of rare earth elements with other elements involves the synthesis and control of multielement systems, so the preparation process and conditions are more complicated [105,106].

Compound Semiconductors Based on Titanium Dioxide
Semiconductor compounding is a method used to enhance photocatalytic efficiency by combining different types of semiconductor materials to form heterojunctions, as exemplified in Figure 8, which depicts a p-n heterojunction formed by TiO2 and ZnO.The semiconductor composite effectively improves photocatalytic efficiency due to the following advantages: 1.By manipulating the size of the modified particles, the spectral absorption range and bandgap of the semiconductor material can be effectively tuned utilizing the quantum size effect [107,108].2. Surface modification of TiO2 plays a role in improving the photostability of the semiconductor materials [109].3. Given that light absorption in semiconductors mainly occurs at the band-edge, the semiconductor composite facilitates more efficient harvesting of sunlight [110].

Titanium Dioxide Composites with Common Semiconductors
Wongburapachart [111] et al. prepared TiO2/NiO-TiO2 bilayer film photocatalyst (BLF) for photocatalytic degradation measurement using acid orange 7 (AO7) solution under light and dark conditions.It was found that compared with ordinary TiO2, the photocatalytic activity of the prepared sample was increased by about 8 times after 48 h of AO7 degradation.Bai [112] et al. synthesized TiO2/ZnO composites by the sol-gel method and the hydrothermal method and found that they have obvious heterostructures, which can reduce the band gap width and improve the light absorption intensity.The photocatalytic mechanism is shown in Figure 9. Ratanathavorn Wittawat et al. [113] prepared TiO2/ZnO composite spherical particles.TiO2/ZnO composite also showed much higher catalytic activity compared to a single component.In addition, Wang et al. [114] also prepared ZnO-TiO2 materials with different composite ratios and found that the specific surface area, pore volume, and pore diameter of ZnO-TiO2 composites were significantly larger than those of TiO2 and the ZnO-TiO2 composites were more surface acidic.The energy band structure facilitates the efficient separation of electrons and holes, and the

Titanium Dioxide Composites with Common Semiconductors
Wongburapachart [111] et al. prepared TiO 2 /NiO-TiO 2 bilayer film photocatalyst (BLF) for photocatalytic degradation measurement using acid orange 7 (AO7) solution under light and dark conditions.It was found that compared with ordinary TiO 2 , the photocatalytic activity of the prepared sample was increased by about 8 times after 48 h of AO7 degradation.Bai [112] et al. synthesized TiO 2 /ZnO composites by the sol-gel method and the hydrothermal method and found that they have obvious heterostructures, which can reduce the band gap width and improve the light absorption intensity.The photocatalytic mechanism is shown in Figure 9. Ratanathavorn Wittawat et al. [113] prepared TiO 2 /ZnO composite spherical particles.TiO 2 /ZnO composite also showed much higher catalytic activity compared to a single component.In addition, Wang et al. [114] also prepared ZnO-TiO 2 materials with different composite ratios and found that the specific surface area, pore volume, and pore diameter of ZnO-TiO 2 composites were significantly larger than those of TiO 2 and the ZnO-TiO 2 composites were more surface acidic.The energy band structure facilitates the efficient separation of electrons and holes, and the catalytic reduction activity and selectivity are stronger.It is further shown that TiO 2 composite with ZnO can inhibit TiO 2 crystal transition and particle growth, and the UV absorption ability is enhanced [115].Abumousa [116] et al. prepared ternary TiO 2 /Y 2 O 3 @g-C 3 N 4 nanocomposites by a simple sonochemical method, which showed excellent photocatalytic properties in the degradation of Congo red dye, Malachite green, and other dyes in aqueous solutions in a short time.These binary semiconductor composites and ternary composites are based on TiO 2 to form heterostructures, and the interface effect and energy band migration in the heterostructures can promote the transfer of photogenerated electrons and holes, thereby improving the rate and efficiency of the photocatalytic reaction.
C3N4 nanocomposites by a simple sonochemical method, which showed excellent photocatalytic properties in the degradation of Congo red dye, Malachite green, and other dyes in aqueous solutions in a short time.These binary semiconductor composites and ternary composites are based on TiO2 to form heterostructures, and the interface effect and energy band migration in the heterostructures can promote the transfer of photogenerated electrons and holes, thereby improving the rate and efficiency of the photocatalytic reaction.TiO2 is composited with other semiconductors to form a composite semiconductor material.This new composite material broadens the excitation wavelengths available to the catalyst, effectively regulates the performance of individual materials, and generates numerous novel photochemical and photophysical properties.In recent years, numerous studies have been conducted on binary semiconductor composites, such as TiO2/ZnO, TiO2/CdS, TiO2/WO3, and ZnO/ZnS, among others.The photocatalytic performance of these compound semiconductors surpasses that of a single semiconductor.

Titanium Dioxide Hybrid Materials with Graphene
In recent years, the modification of graphene composite TiO2 has become the focus of many researchers.Graphene with a two-dimensional structure has a large number of twodimensional conjugated structures, so people combine graphene with TiO2 to enhance the photocatalytic performance of TiO2, which has been extensively studied in this area.Heltina [117], Wang [118], and others prepared TiO2 with different graphene (GO) composite ratios compared to the pure TiO2 and the composite TiO2/GO catalysts.The smaller grain size and higher adsorbed oxygen/lattice oxygen ratio exhibited superior photocatalytic performance.In addition, GO acts as a capture center for photogenerated electrons and transfers electrons to the target reactants, thus inhibiting the recombination rate of photogenerated electron-hole pairs and increasing the photocatalytic rate of TiO2.However, graphene tends to aggregate in solution to form clusters, which can lead to difficulties in controlling the homogeneity and dispersion of graphene in the composites [119], and the preparation of composites of titanium dioxide and graphene usually requires special synthesis techniques and equipment, which may lead to high preparation costs.This makes these composites difficult to commercialize on a large scale for some applications.TiO 2 is composited with other semiconductors to form a composite semiconductor material.This new composite material broadens the excitation wavelengths available to the catalyst, effectively regulates the performance of individual materials, and generates numerous novel photochemical and photophysical properties.In recent years, numerous studies have been conducted on binary semiconductor composites, such as TiO 2 /ZnO, TiO 2 /CdS, TiO 2 /WO 3 , and ZnO/ZnS, among others.The photocatalytic performance of these compound semiconductors surpasses that of a single semiconductor.

Titanium Dioxide Hybrid Materials with Graphene
In recent years, the modification of graphene composite TiO 2 has become the focus of many researchers.Graphene with a two-dimensional structure has a large number of two-dimensional conjugated structures, so people combine graphene with TiO 2 to enhance the photocatalytic performance of TiO 2 , which has been extensively studied in this area.Heltina [117], Wang [118], and others prepared TiO 2 with different graphene (GO) composite ratios compared to the pure TiO 2 and the composite TiO 2 /GO catalysts.The smaller grain size and higher adsorbed oxygen/lattice oxygen ratio exhibited superior photocatalytic performance.In addition, GO acts as a capture center for photogenerated electrons and transfers electrons to the target reactants, thus inhibiting the recombination rate of photogenerated electron-hole pairs and increasing the photocatalytic rate of TiO 2 .
However, graphene tends to aggregate in solution to form clusters, which can lead to difficulties in controlling the homogeneity and dispersion of graphene in the composites [119], and the preparation of composites of titanium dioxide and graphene usually requires special synthesis techniques and equipment, which may lead to high preparation costs.This makes these composites difficult to commercialize on a large scale for some applications.

TiO 2 Composite Polymers
Combining modified TiO 2 with polymers can endow nanocomposite materials with new properties.Additionally, polymers can enhance the adsorption and photocatalytic performance of nano-TiO 2 , facilitating its separation and recovery [120].
Maeda et al. [121] first employed a phosphorus coupling agent to modify the surface of the modified TiO 2 particles, aiming to enhance their compatibility with specific organic monomers (Figure 10).TiO 2 @PMMA hybrids were successfully obtained through in situ polymerization.It can be observed that as the in situ polymerization time elongates, the PMMA polymer chains growing on the surface of TiO 2 particles lead to an increase in the distance between the nanoparticles, thereby enhancing the transparency of the PMMA composites.This method maintains the flexibility, film forming, and electrical conductivity of the polymer.In addition, the composite may also exhibit better photocatalytic activity and antimicrobial properties.monomers (Figure 10).TiO2@PMMA hybrids were successfully obtained through in situ polymerization.It can be observed that as the in situ polymerization time elongates, the PMMA polymer chains growing on the surface of TiO2 particles lead to an increase in the distance between the nanoparticles, thereby enhancing the transparency of the PMMA composites.This method maintains the flexibility, film forming, and electrical conductivity of the polymer.In addition, the composite may also exhibit better photocatalytic activity and antimicrobial properties.Interestingly, Shi et al. [122] first coated stearic acid on the surface of TiO2 particles by impregnation method and then further modified it with paraffin wax to prepare TiO2 with Janus structure, which enhances the surface charge separation efficiency and adsorption capacity of organic matter (Figure 11).In addition, the modified Janus-like TiO2 can be used as an additive to stabilize Pickering emulsion, which in turn enhances its efficiency in degrading oil-phase pollutants in high-concentration kerosene and nitrobenzene wastewater.Interestingly, Shi et al. [122] first coated stearic acid on the surface of TiO 2 particles by impregnation method and then further modified it with paraffin wax to prepare TiO 2 with Janus structure, which enhances the surface charge separation efficiency and adsorption capacity of organic matter (Figure 11).In addition, the modified Janus-like TiO 2 can be used as an additive to stabilize Pickering emulsion, which in turn enhances its efficiency in degrading oil-phase pollutants in high-concentration kerosene and nitrobenzene wastewater.monomers (Figure 10).TiO2@PMMA hybrids were successfully obtained through in situ polymerization.It can be observed that as the in situ polymerization time elongates, the PMMA polymer chains growing on the surface of TiO2 particles lead to an increase in the distance between the nanoparticles, thereby enhancing the transparency of the PMMA composites.This method maintains the flexibility, film forming, and electrical conductivity of the polymer.In addition, the composite may also exhibit better photocatalytic activity and antimicrobial properties.Interestingly, Shi et al. [122] first coated stearic acid on the surface of TiO2 particles by impregnation method and then further modified it with paraffin wax to prepare TiO2 with Janus structure, which enhances the surface charge separation efficiency and adsorption capacity of organic matter (Figure 11).In addition, the modified Janus-like TiO2 can be used as an additive to stabilize Pickering emulsion, which in turn enhances its efficiency in degrading oil-phase pollutants in high-concentration kerosene and nitrobenzene wastewater.Nair [123] et al. fixed PANI-TiO 2 nanocomposites in polystyrene cubes to form PANi-TiO 2 @polystyrene cubes for photocatalytic degradation of acid yellow 17 (AY 17) dyes under visible light.And the photocatalytic activity was significantly improved.It provides a way to prepare more excellent new photocatalysts.Tran et al. [124] formulated different concentrations of acrylic acid (AA) mixed with isopropanol to modify the nano-TiO 2 and then uniformly coated it on the surface of polyvinylidene fluoride (PVDF) film.At high temperatures, AA reacts with PVDF, and nano-TiO 2 is fixed on the surface of the film to maintain its flexibility and film formation, which can improve the photocatalytic activity of the composite.Neves et al. [125] used polydimethylsiloxane-modified TiO 2 nanoparticles to increase the surface roughness, enhance their hydrophobic strength and photocatalytic activity, and provide ideas for achieving complete degradation of polymers.

Summary and Outlook
In recent years, significant progress has been made in the field of TiO 2 modified photodegradation of organic pollutants.Through a series of modification methods, the photocatalytic performance of TiO 2 has been significantly improved, providing a more efficient and reliable solution for the photodegradation process of organic pollutants.The following is a summary of the research progress in this field in recent years, including prospects of future research development.

•
By doping precious metals, transition metals, rare earth metals, or non-metallic elements, TiO 2 can change the band structure, broaden its light absorption range, and improve the separation efficiency of photoelectron-hole pairs, which can significantly improve the photocatalytic activity of TiO 2 .• TiO 2 was mixed with other semiconductor materials to form a composite photocatalytic material with a heterogeneous structure.This modification method can make use of the synergistic effect between different materials to improve the utilization efficiency of photogenerated electron-hole pairs and enhance photocatalytic performance.For example, the composite of TiO 2 with SiO 2 , ZnO, and other materials can form heterogeneous structures and improve photocatalytic efficiency.

•
By introducing functional material polymer on the surface of TiO 2 , the surface properof TiO 2 are improved, and the photocatalytic performance is improved.Surface modification can increase the active sites on the surface of TiO 2 and promote the separation and migration of photogenerated electrons and holes.
The five modification methods mentioned in this paper, the dopants commonly used, the specific surface area, the band gap energy, and degradation effects of the modified TiO 2 photocatalyst are shown in Table 2.The degradation rate of Dianix blue dye reached 91%.[139] Polydopamine (PDA) --3.22~3.15 The photocatalytic CO 2 reduction yield of CH 4 by the composite was up to 1.50 µmol/g•h, which was 5 times that of pure TiO 2 . [140] In summary, the modified TiO 2 photocatalyst significantly improves its photocatalytic performance in UV and visible light by increasing the specific surface area and reducing the band gap energy.The larger specific surface area increases the catalyst's active site and improves the contact efficiency with pollutant molecules, while the reduced band gap energy enables the catalyst to absorb a wider spectrum, including visible light, thereby broadening the photoresponse range and enhancing the utilization of sunlight.In addition, the specific modification method can further promote the separation and migration of photogenerated electrons and holes and further improve photocatalytic efficiency.These improvements make the modified TiO 2 photocatalyst show a broader application potential in the field of environmental governance and new energy development.
The photocatalytic performance of TiO 2 was improved to varying degrees.However, due to problems such as low efficiency, insufficient stability, and secondary pollution, TiO 2 modification methods cannot be widely used.The advantages and disadvantages of TiO 2 modification methods are shown in Table 3.The complexity of design and preparation.
TiO 2 composite polymers More environmentally friendly; Mechanical properties will be improved; Can be repeated many times.
The dispersion is not good; May degrade the polymer matrix.

Future Research Direction and Development Trend
Although TiO 2 modified photodegradation of organic pollutants has made remarkable progress, there are still some key problems and shortcomings.First, the stability of the modification effect is still a challenge, which can lead to performance fluctuations in practical applications.Secondly, the high preparation cost limits the possibility of large-scale applications.Therefore, future research needs to further explore and optimize modification methods to improve their stability and reduce costs.
In addition, the importance of mechanism research cannot be ignored.Strengthening the mechanism study can not only provide solid theoretical support for the optimization of modification methods but also help us to understand more deeply the reaction mechanism of TiO 2 photocatalytic degradation of organic pollutants.This will lay the foundation for the design of more efficient and stable TiO 2 photocatalytic materials.
In practical applications, the effect of TiO 2 photocatalytic degradation of organic pollutants may be affected by a variety of factors, including water quality, light conditions, dye type, and concentration.Therefore, future research also needs to focus on how to optimize the performance of TiO 2 photocatalytic degradation of organic pollutants in various real-world environments.
In conclusion, optimizing the preparation method and process of TiO 2 composite photocatalytic materials has become an important direction of future research on the photodegradation of organic pollutants.By introducing visible light absorbing inorganic substances or modifying TiO 2 , we can prepare multi-functional composite materials that can expand the range of light absorption and, at the same time, play the role of photocatalysis, adsorption, and catalysis, thus significantly improving the degradation efficiency of organic matter.With continuous research and exploration, we look forward to developing more efficient, stable, and environmentally friendly TiO 2 photocatalytic materials, making important contributions to environmental protection and sustainable development.

Figure 3 .
Figure 3. Schematic diagram of TiO2 preparation process by sol-gel method.

Figure 3 .
Figure 3. Schematic diagram of TiO 2 preparation process by sol-gel method.

Figure 6 .
Figure 6.Schematic diagram of electron transfer in the noble metal deposition system [67].

Figure 6 .
Figure 6.Schematic diagram of electron transfer in the noble metal deposition system [67].

TiO 2 -
doped transition metalThe presence of polyvalent transition metals promotes chemical reactions, modulates the electronic structure of TiO 2 to improve its photocatalytic properties, and extends the light absorption range.Prone to focusing; not environmentally friendly.TiO 2 -doped rare earth metals Good stability; high catalytic activity; expanding the range of TiO 2 light absorption and promoting photocatalytic reactions.Complicated operating procedures; not easy to recycle.TiO 2 compound semiconductors Formation of heterojunctions to expand the light absorption range of the material and improve photocatalytic efficiency.Reduction in electron-hole complex reaction.

Table 1 .
Reaction Principle of TiO 2 Photocatalyst Common Preparation Methods and Their Advantages and Disadvantages.

Table 2 .
Characterization and degradation effect of modified TiO 2 photocatalyst.

Table 3 .
Advantages and disadvantages of TiO 2 modification methods.